Advances in Materials 2017; 6(6): 102-114 http://www.sciencepublishinggroup.com/j/am doi: 10.11648/j.am.20170606.11 ISSN: 2327-2503 (Print); ISSN: 2327-252X (Online) Nitrate Removal from Groundwater Using Sodium Alginate Doped with Nano-Hydroxyapatite Salah Abo-El-Enein 1 , Yahia Gedamy 2, * , Amr Ecresh 3 1 Chemistry Department, Faculty of Science, Ain Shams University, Cairo, Egypt 2 Hydrogeochemistry Department, Desert Research Center, Cairo, Egypt 3 North and South Sinai Company for Water and Wastewater, Sinai Peninsula, Egypt Email address: [email protected] (Y. Gedamy) * Corresponding author To cite this article: Salah Abo-El-Enein, Yahia Gedamy, Amr Ecresh. Nitrate Removal from Groundwater Using Sodium Alginate Doped with Nano- Hydroxyapatite. Advances in Materials. Vol. 6, No. 6, 2017, pp. 102-114. doi: 10.11648/j.am.20170606.11 Received: March 16, 2017; Accepted: April 12, 2017; Published: October 26, 2017 Abstract: In the present work, the hydroxyapatite/alginate nano-composite adsorbent was prepared by incorporating nano- sized hydroxyapatite (nHAp) into alginate polymer and uses this adsorbent for removal of nitrate from groundwater. The synthesized nano-composite and pure alginate as well as the pure hydroxyapatite were characterized with Fourier Transform Infrared (FT-IR) spectroscopy to ascertain the functional groups. The adsorption characteristics of nitrate from groundwater on the HAp/Alg nano-composite were optimized under different operational parameters like contact time, pH, adsorbent dosage, initial concentration of nitrate and temperature in batch system. Maximum equilibrium capacity reached 99% of nitrate removal by using the HAp/Alg nano-composite after 240min at pH 3; adsorbent dosage, 2g; initial concentration, 100mg/l and temperature, 20°C. The kinetics studies revealed that the pseudo-second-order kinetic model was able to describe the dynamic behavior of the adsorption process by composite adsorbents used in this work. Also, the Langmuir isotherm model is very well fitted to the equilibrium data. The mechanism of NO 3 - ions adsorption by the nano-composite adsorbent was described. So, it is concluded that HAp/Alg nano-composite is a relatively efficient and low cost as well as the results validated the feasibility of HAp/Alg nano-composite for highly effective removal of nitrate from an aqueous solution. Keywords: Nitrate, Hydroxyapatite/Alginate Nano-Composite, Groundwater 1. Introduction Assiut governorate, one of the oldest governorates of Upper Egypt, It extends south-north between Sohag and El- Minya governorates from latitude 26° 47 ' N to 27° 37 ' N and extends west-east between New Valley and Red Sea governorates from longitudes 30° 37 ' E to 31° 34 ' E (Figure 1). The total Assiut governorate area is 25,926km², equivalent to about 2.6% of the total area of Egypt. The extension of the River Nile along study area is about 120km while the width of the study area ranges between 10 and 20km (ALDAR, 2011). Estimated population of the Assiut governorate is about 4,245,215 million (Census estimation, 2015), representing 4.8% of Egypt's total population. Groundwater quality assessment is considered as a significant topic to make sure possible safe use of this resource. As the population continues to increase, it is necessary to find additional sources of water such as groundwater. Groundwater is deemed one of the major resources for potable water in Assiut governorate especially in rural areas (ALDAR, 2011). In this study, selected samples of groundwater were collected and chemically analyzed. Analysis of these samples (Table 1) revealed that they have nitrate concentrations more than the maximum permissible limit recommended (50mg/l) by WHO, 2011. This is due its high solubility in water and this is manifested by Hekmatzadeh et al., 2012, who state that due to its high solubility, nitrate is the most likely cause of the contamination in groundwater across the globe, and a potential threat to water resource, as well as increasing eutrophication. Nitrate contamination in drinking water sources has been a
Advances in Materials 2017; 6(6): 102-114
ISSN: 2327-2503 (Print); ISSN: 2327-252X (Online)
Nitrate Removal from Groundwater Using Sodium Alginate Doped with Nano-Hydroxyapatite
Salah Abo-El-Enein1, Yahia Gedamy
2, *, Amr Ecresh
1Chemistry Department, Faculty of Science, Ain Shams University, Cairo, Egypt 2Hydrogeochemistry Department, Desert Research Center, Cairo, Egypt 3North and South Sinai Company for Water and Wastewater, Sinai Peninsula, Egypt
The suitability of HAp/Alg nano-composite was tested
with a field samples taken from the study area. About 2g
of adsorbent was added to 50ml of water sample and the
contents were shaken with constant time 240min at room
temperature. As shown in table (4), the results indicated
that the removal percentage reached about 99%, which
reveal that HAp/Alg adsorbent nano-composite can be
effectively employed for removing the nitrate ion from
Table 4. Field trial results of HAp/Alg nano-composite on groundwater samples at the study area.
Sample No. Nitrate concentration before treatment Nitrate concentration after treatment Removal percentage (%)
1 57.75 0.51 99.12
2 65.13 0.6 99.07
3 74.18 0.75 98.99
This study demonstrated how the nHAp/Alg nano-
composite prepared and employed for the removal of nitrate
ions from groundwater in a batch method, can be used as a
more effective adsorbent in use. The alginate gel is prepared
by diffusion method or gelation method when a calcium salt
is added to a solution of sodium alginate in water. In gelation
method, the crosslinking calcium ion diffuses from an outer
reservoir into an alginate solution and the gel forms by a
chemical reaction, the calcium displaces the sodium from the
alginate, holds the long alginate molecules together and a gel
is resulted. No heat is required and the gel does not melt
when heated. The HAp/Alg nano-composite adsorbent was
synthesized by in situ hybridization. The FT-IR spectroscopy
results indicate that there is a chemical interaction takes place
between the inorganic and polymeric constituents in the
composite. The chemical interaction is assumed to be
mediated by the chemical bonding between Ca2+
carboxyl groups in alginate. Maximum equilibrium capacity
is 99% of nitrate removal was obtained using the HAp/Alg
nano-composite after 240min; at pH, 3; adsorbent dosage, 2g,
initial concentration, 100mg/l and temperature 20°C. The
kinetics of nitrate adsorption onto the nHAp/Alg nano-
composite revealed that nitrate ions adsorbed satisfactorily,
according to the pseudo second-order equation. Fitting of the
kinetic data of the adsorbent nHAp/Alg to pseudo second-
order indicates that the concentration of both adsorbate and
adsorbent are involved in the rate determining step of the
adsorption process. Also, the Langmuir isotherm model fitted
the equilibrium data better than the Freundlich isotherm,
which demonstrated homogeneous surface with monolayer of
adsorbate. The process can be employed for the removal of
nitrate to meet the permissible limit of nitrate for human
drinking water in both surface and groundwater. Finally, the
beads type nHAp–alginate composite adsorbent was found to
be promising for nitrate ions removal from aqueous
 Akçelik, O.; Tosun, A. and Ergun, M., 2008. Biosorption of copper (ii) from aqueous solution by Saccharomyces cerevisiae, 4th European Bioremediation Conference, Greece.
 ALDAR, CH2M Hill, Spain, 2011. Study of environmental and social impact assessment framework (ESIAF) of Assiut & Sohag governorates. Executive Summary, Egypt, 82p.
 Annadurai, G. and Krishnan M. R. V., 1996. Adsorption of basic dye using chitin. Indian J Environ Protec. 16 (6): 444-449.
113 Salah Abo-El-Enein et al.: Nitrate Removal from Groundwater Using Sodium Alginate Doped with Nano-Hydroxyapatite
 Arica, M. Y.; Arpa, C.; Ergene, A.; Bayramoglu, G. and Genc, O., 2003. Ca–alginate as a support for Pb(II) and Zn(II) biosorption with immobilized Phanerochaete chrysosporium, Carbohydr. Polym., 52: 167–174.
 Cantor, K. P., 1997. Drinking water and cancer. Cancer Causes Control, 8: 292–308.
 Census estimation, 2015. Estimation of Central Agency for Public Mobilization and Statistics, 2015 (in Arabic).
 Do˘gan, M. and Alkan, M., 2003. Adsorption kinetics of methyl violet onto perlite. Chemosphere, 50 (4), 517-528.
 Dorsche, M. M.; Scragg, R. K. R.; McMichael, A. J.; Baghurst, P. A. and Duer, K. F., 1984. Congenital malformation and maternal drinking water supplying rural South Australia: a case study. Am. J. Epidemiol., 119: 473–486.
 Elmoubarki, R.; Mahjoubi, F. Z.; Tounsadi, H.; Moustadraf, J.; Abdennouri, M.; Zouhri, A.; ElAlbani, A. and Barka, N., 2015. Adsorption of textile dyes on raw and decanted Moroccan clays: Kinetics, Equilibrium and Thermodynamics. Water Resources and Industry, 9: 16-29.
 Fahimeh Googerdchian; Ahmad Moheb and Rahmatollah Emadi, 2012. Lead sorption properties of nanohydroxyapatite–alginate composite adsorbents. Chemical Eng. J., 200, 202: 471–479.
 Ganjali, M. R.; Babaei, L. H.; Norouzi, P.; Pourjavid, M. R.; Badiei, A.; Saberyan, K.; Maragheh, M. G.; Salavati-Niasari, M. and Ziarani, G. M., 2005. Novel method for the fast separation and purification of molybdenum (VI) from fission products of uranium with aminofunctionalized mesoporous molecular sieves (AMMS) modified by dicyclohexyl-18-crown-6 and S-N tetradentate Schiff’s base. Analytical Letters, 38 (11): 1813–1821.
 Grant, G. T.; Morris, E. R.; Rees, D. A.; Smith, P. J. and Thom, D., 1973. Biological interaction between polysaccharides and di-valent cations. The egg-box model. FEBS Lett, 32: 195–198.
 Hekmatzadeh, A. A.; Karimi-Jashani, A.; Talebbeydokhti, N. and Kløve, B., 2012. Modeling of nitrate removal for ion exchange resin in batch and fixed bed experiments, J. Desalination, 284: 22–31.
 Ho, Y. S. and McKay, G., 1999. Pseudo-second order model for sorption processes, Process Biochem. 34: 451–465.
 Ho, Y.; Porter, J. and McKay, G., 2002. Equilibrium isotherm studies for the sorption of divalent metal ions onto peat: copper, nickel and lead single component systems. Water, Air & Soil Pollution, 141 (1–4): 1–33.
 Honghe, Z., 1997. Interaction mechanism in sol–gel transition of alginate solutions by addition of divalent cations. Carbohydr. Res., 302: 97–101.
 Ingleton, I. and Simmons, P., 1996. Factors affecting silver biosorption by an industrial strain of Saccharomyces cerevisiae. J. Chem. Technol. Biotechnol., 65: 21-28.
 Islam, M. and Patel, R., 2011. Physicochemical characterization and adsorption behavior of Ca/Al chloride hydrotalcite - like compound towards removal of nitrate. J. Hazard. Mater. 190: 659-668.
 Jae-HeeAhn; Kwang-Ho Choo and Hak-Soon Park, 2008. Reverse osmosis membrane treatment of acidic etchant
wastewater: Effect of neutralization and polyelectrolyte coating on nitrate removal, J. Membrane Sci., 310: 296–302.
 Kapoor, A. and Viraraghavan, T., 1997. Nitrate removal from drinking water—review. J. Environ. Eng., 123: 371 – 380.
 Kar, S.; Khan, D. K. and Santra, S. C., 2002. Groundwater nitrate concentration and its impact on human health: a review. Every man’s Sci., 37: 35–40.
 Kesseru, P.; Kiss, I.; Bihari, Z. and Polyak, B., 2002. Investigation of the denitrification activity of immobilized Pseudomonas butanovora cells in the presence of different organic substrates. Water Res., 36: 1565–1571.
 Kikuchi, M.; Itoh, S.; Ichinose, S.; Shinomiya, K. and Tanaka, J., 2001. Self-organization mechanism in a bone-like hydroxyapatite / collagen nano-composite synthesized in vitro and its biological reaction in vivo. Biomaterials, 22: 1705–1711.
 Komath, M. and Varma, H. K., 2003. Development of a fully injectable calcium phosphate cement for orthopedic and dental applications. Bull. Mater. Sci., 26 (4): 415-422.
 Mahamudur Islam; Prakash Chandra Mishra and Rajkishore Patel, 2010. Physicochemical characterization of hydroxyapatite and its application towards removal of nitrate from water. J. Environ. Manage., 91: 1883-1891.
 Malberg, J. W.; Savage, E. P. and Osteryoung, J., 1978. Nitrate in drinking water and the early onset of hypertension. Environ. Pollut., 15: 155–161.
 McKay, G., 1983. The adsorption of dye stuff from aqueous solution using activated carbon: analytical solution for batch adsorption based on external mass transfer and pore diffusion. Chem. Eng. J., 27:187.
 McKay, G.; Otterburn, M. S. and Aja, J. A., 1985. Fullter’s earth and fired clay as adsorbents for dyes stuffs. Water Air Soil Pollut. 24: 307.
 Mishra, P. C. and Patel, R. K., 2009. Use of agricultural waste for the removal of nitrate-nitrogen from aqueous medium, J. Environ. Manage., 90: 519-522.
 Mohammad Hassan Shahmoradi; Behnoush Amin Zade; Ali Torabian and Mahdi Seyed Salehi, 2015. Removal of nitrate from groundwater using activated carbon prepared from rice husk and sludge of paper industry wastewater treatment. ARPN J. Eng. and Applied Sci., 10 (17): 7856-7863.
 Morey, M. S.; O’Brien, S.; Schwarz, S. and Stucky, G. D., 2000. Hydrothermal and post-synthesis surface modification of cubic, MCM-48 and ultra large pore SBA-15 mesoporous silica with titanium. Chemi. of Materi. J., 12 (4): 898–911.
 Moussavi, G. and Khosravi, R., 2011. The removal of cationic dyes from aqueous solutions by adsorption onto Pistachio Hull Waste. Chemical Eng. Res. and Design J., 89: 2182-2189.
 Nayak, D. and Lahiri, S., 2006. Biosorption of toxic, heavy, no-carrier-added radionuclides by calcium alginate beads, J. Radioanal. Nucl. Chem., 267: 59–65.
 Prakasa Rao, E. V. S. and Puttanna, K., 2000. Nitrates, agriculture and environment. Current Sci., 79: 1163–1168.
 Ravikrishna, R.; Ren, M. and Valsaraj, K. T., 2006. Low-temperature synthesis of porous hydroxyapatite scaffolds using polyaphron templates, J. Sol–Gel Sci. Technol., 38: 203–210.
Advances in Materials 2017; 6(6): 102-114 114
 Ruiz-Hitzky, E., 2003. Functionalizing inorganic solids: towards organic–inorganic nanostructured materials for intelligent and bio-inspired systems. The Chemical Record, 88–100.
 Ryker, S. J. and Jones, J. L., 1995. Nitrate concentrations in groundwater of the central Columbia plateau. U.S. Geological Survey Fact Sheet, FS-061-97.
 Sachin N. Milmile; Jayshri V. Pande; Shilpi Karmakar; Amit Bansiwal; Tapan Chakrabarti and Rajesh B. Biniwale, 2011. Equilibrium isotherm and kinetic modeling of the adsorption of nitrates by anion exchange Indion NSSR resin, Desalination, 276: 38–44.
 Sefner, W., 1995. Natural water contents and endemic goiter—a review. Zentralb. Hyg. Umweltmed., 196: 381–398.
 Selvam, P.; Bhatia, S. K. and Sonwane, C. G., 2001. Recent advances in processing and characterization of periodic mesoporous MCM-41 silicate molecular sieves. Indus. & Eng. Chemi. Res. J., 40 (15): 3237–3261.
 Sheridan, M. H.; Shea, L. D.; Peters, M. C. and Mooney, D. J., 2000. Bioabsorbable polymer scaffolds for tissue engineering capable of sustained growth factor delivery. J. Control Release, 64: 91–102.
 Soumya, G. N.; Manickavasagam, M.; Santhanam, P.; Dinesh Kumar, S. and Prabhavathi, P., 2015. Removal of phosphate and nitrate from aqueous solution using seagrass Cymodocea rotundata beads. African J. Biotechno. 14 (16): 1393-1400.
 Sudipta Chatterjee; Dae S. Leeb; Min W. Leec and Seung H. Woo., 2009. Nitrate removal from aqueous solutions by cross-linked chitosan beads conditioned with sodium bisulfate, J. Hazard. Mater., 166: 508–513.
 Super, M.; Heese, H.; Machenzie, D.; Dempster, W. S.; Duplers, J. and Ferreina, J. J., 1981. An epidemiological study of well water nitrates in a group of southwest African/Namibian infants. Water Res., 15: 1265–1270.
 Sutherland, I. W., 1991. Alginates. In: Byron D, editor. Biomaterials: novel materials from biological sources. New York: Stockton Press, 309–331.
 Suriyaraj, S. P. and R. Selvakumar, 2016. Advances in nanomaterial based approaches for enhanced fluoride and nitrate removal from contaminated water. RSC Adv., 6: 10565-10583.
 Tahir, H., 2005. Comparative trace metal contents in sediments and liquid waste from tanneries and their removal of chromium using Zeolite-5A. Electronic J. Environ., Agricultural and Food Chemistry, EJEAFCHE 4 (4): 1021-1032.
 Teng, S.; Shi, J.; Peng, B. and Chen, L., 2006. The effect of alginate addition on the structure and morphology of hydroxyapatite gelatin nano-composites. Compos. Sci. Technol., 66:1532–1538.
 Van Maanen, J. M. S.; Van Dijk, A.; Mulder, K.; De Baets, M. H.; Menheere, P. C. A.; Van Der Heide, D.; Mertens, P. L. J. M. and Kleinjans, J. C. S., 1994. Consumption of drinking water with high nitrate levels causes hypertrophy of the thyroid. Toxicol. Lett., 72: 365–374.
 Vimonses, V.; Lei, S.; Jin, B.; Chow, C. W. K. and Saint, C., 2009. Adsorption of Congo Red by three Australian kaolin's. Applied Clay Sci. J., 43: 465-472.
 Wahab, M. A.; Jellali, S. and Jedidi, N., 2010. Effect of temperature and pH on the biosorption of ammonium onto Posidonia oceanica fibers: Equilibrium, and kinetic modeling studies. Bioresour. Technol., 101: 8606-8615.
 Wang, Z.; Zhang, Q.; Konno, M. and Saito, S., 1993. Sol-gel transition of alginate solution by the addition of various divalent cations: 13C-NMR spectroscopic study. Biopolymers, 33:703–711.
 Wang, Li.; Yue, Li. and Chunzhong, Li., 2009. In situ processing and properties of nanostructured hydroxyapatite / alginate composite. J. Nanopart. Res., 11: 691–699.
 Weber, Jr. W. J., 1972. Physico-chemical processes for water quality control. New York: Wiley Interscience, 27: (Chapter 5) 207–234.
 Weber, W. J. and Morris, J. C., 1964. In: Eckenfelder, W. W, editor. Advances in water pollution research. Oxford: Pergamom Press.
 WHO, 2011. Guidelines for drinking-water quality. Recommendations. 4th ed. Geneva, World Health Organization. ISBN 978 92 4 154815 1.
 Yadav, A. K.; Kaushik, C. P.; Haritash, A. K.; Kansal, A. and Rani, N., 2006. Defluoridation of groundwater using brick powder as an adsorbent. J. Hazard. Mater. 128: 289-293.
 Yuh-Shan Ho., 2005. Comment on “Nitrate removal from aqueous solution by adsorption onto various materials” by N. O¨ ztu¨rk, T. E. Bektas, J. Hazard. Mater., B, 118: 253–254.
 Zhang, J.; Wang, Q. and Wang, A., 2010. In situ generation of sodium alginate/hydroxyapatite nano-composite beads as drug-controlled release matrices. Acta Biomaterial, 6: 445–454.